#------------------------------------------------------------------------------
#$Date: 2016-02-20 05:06:23 +0200 (Sat, 20 Feb 2016) $
#$Revision: 176774 $
#$URL: svn://www.crystallography.net/cod/cif/2/20/76/2207684.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2207684
loop_
_publ_author_name
'Kończyk, J.'
'Demchenko, P.'
'Demchenko, G.'
'Bodak, O.'
'Marciniak, B.'
_publ_section_title
;
 Erbium nickel trisilicide, ErNiSi₃
;
_journal_coeditor_code           WM6110
_journal_issue                   12
_journal_name_full               'Acta Crystallographica Section E'
_journal_page_first              i259
_journal_page_last               i261
_journal_paper_doi               10.1107/S160053680503566X
_journal_volume                  61
_journal_year                    2005
_chemical_formula_iupac          'Er Ni Si3'
_chemical_formula_moiety         'Er Ni Si3'
_chemical_formula_sum            'Er Ni Si3'
_chemical_formula_weight         310.24
_chemical_name_common            'Erbium Nickel Trisilicide'
_chemical_name_systematic
;
Erbium Nickel Trisilicon
;
_space_group_IT_number           65
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-C 2 2'
_symmetry_space_group_name_H-M   'C m m m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   3.9152(5)
_cell_length_b                   20.948(3)
_cell_length_c                   3.9313(6)
_cell_measurement_reflns_used    1395
_cell_measurement_temperature    295(2)
_cell_measurement_theta_max      32.72
_cell_measurement_theta_min      5.19
_cell_volume                     322.43(8)
_computing_cell_refinement       'CrysAlis CCD'
_computing_data_collection       'CrysAlis CCD (Oxford Diffraction, 2004)'
_computing_data_reduction        'CrysAlis RED (Oxford Diffraction, 2005)'
_computing_molecular_graphics    'DIAMOND (Brandenburg, 1999)'
_computing_publication_material  'SHELXL97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      295(2)
_diffrn_measured_fraction_theta_full 0.980
_diffrn_measured_fraction_theta_max 0.947
_diffrn_measurement_device_type  'Oxford Diffraction Xcalibur3 CCD'
_diffrn_measurement_method       ω
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0279
_diffrn_reflns_av_sigmaI/netI    0.0178
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       30
_diffrn_reflns_limit_k_min       -30
_diffrn_reflns_limit_l_max       5
_diffrn_reflns_limit_l_min       -3
_diffrn_reflns_number            1407
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         32.72
_diffrn_reflns_theta_min         5.19
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    32.504
_exptl_absorpt_correction_T_max  0.2743
_exptl_absorpt_correction_T_min  0.1867
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details   'CrysAlis RED (Oxford Diffraction, 2005)'
_exptl_crystal_colour            'metallic light grey'
_exptl_crystal_density_diffrn    6.391
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             552
_exptl_crystal_size_max          0.070
_exptl_crystal_size_mid          0.045
_exptl_crystal_size_min          0.040
_refine_diff_density_max         1.373
_refine_diff_density_min         -1.366
_refine_ls_extinction_coef       0.0108(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL97
_refine_ls_goodness_of_fit_ref   1.020
_refine_ls_matrix_type           full
_refine_ls_number_parameters     22
_refine_ls_number_reflns         360
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.020
_refine_ls_R_factor_all          0.0166
_refine_ls_R_factor_gt           0.0163
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w = 1/[σ²(Fo²)+(0.0156P)²+8.1601P] where P = (Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0396
_refine_ls_wR_factor_ref         0.0398
_reflns_number_gt                358
_reflns_number_total             360
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            wm6110.cif
_cod_data_source_block           I
_cod_original_cell_volume        322.42(8)
_cod_database_code               2207684
_cod_database_fobs_code          2207684
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, -z'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, z'
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
_atom_site_type_symbol
Er 0.0000 0.331215(13) 0.5000 0.00485(12) Uani d S 1 Er
Ni 0.0000 0.11061(4) 0.0000 0.00510(16) Uani d S 1 Ni
Si1 0.0000 0.05585(9) 0.5000 0.0071(3) Uani d S 1 Si
Si2 0.0000 0.21787(9) 0.0000 0.0054(3) Uani d S 1 Si
Si3 0.0000 0.44397(9) 0.0000 0.0067(3) Uani d S 1 Si
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Er Er -0.2586 4.9576 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
Si2 Er Si2 13_455 13_556 139.32(7) n
Si2 Er Si2 13_455 13_456 83.27(3) n
Si2 Er Si2 13_556 13_456 82.85(2) n
Si2 Er Si2 13_455 13 82.85(2) n
Si2 Er Si2 13_556 13 83.27(3) n
Si2 Er Si2 13_456 13 139.32(7) n
Si2 Er Ni 13_455 13_556 176.63(4) n
Si2 Er Ni 13_556 13_556 44.05(4) n
Si2 Er Ni 13_456 13_556 97.831(18) n
Si2 Er Ni 13 13_556 98.239(17) n
Si2 Er Ni 13_455 13_455 44.05(4) n
Si2 Er Ni 13_556 13_455 176.63(4) n
Si2 Er Ni 13_456 13_455 98.239(17) n
Si2 Er Ni 13 13_455 97.831(17) n
Ni Er Ni 13_556 13_455 132.57(3) n
Si2 Er Ni 13_455 13_456 98.239(17) n
Si2 Er Ni 13_556 13_456 97.831(17) n
Si2 Er Ni 13_456 13_456 44.05(4) n
Si2 Er Ni 13 13_456 176.63(4) n
Ni Er Ni 13_556 13_456 80.493(15) n
Ni Er Ni 13_455 13_456 80.892(15) n
Si2 Er Ni 13_455 13 97.831(18) n
Si2 Er Ni 13_556 13 98.239(17) n
Si2 Er Ni 13_456 13 176.63(4) n
Si2 Er Ni 13 13 44.05(4) n
Ni Er Ni 13_556 13 80.892(15) n
Ni Er Ni 13_455 13 80.493(15) n
Ni Er Ni 13_456 13 132.57(3) n
Si2 Er Si1 13_455 13_556 133.60(3) n
Si2 Er Si1 13_556 13_556 81.14(3) n
Si2 Er Si1 13_456 13_556 133.60(3) n
Si2 Er Si1 13 13_556 81.14(3) n
Ni Er Si1 13_556 13_556 43.803(15) n
Ni Er Si1 13_455 13_556 95.86(2) n
Ni Er Si1 13_456 13_556 95.86(2) n
Ni Er Si1 13 13_556 43.803(15) n
Si2 Er Si1 13_455 13_456 81.14(3) n
Si2 Er Si1 13_556 13_456 133.60(3) n
Si2 Er Si1 13_456 13_456 81.14(3) n
Si2 Er Si1 13 13_456 133.60(3) n
Ni Er Si1 13_556 13_456 95.86(2) n
Ni Er Si1 13_455 13_456 43.803(15) n
Ni Er Si1 13_456 13_456 43.803(15) n
Ni Er Si1 13 13_456 95.86(2) n
Si1 Er Si1 13_556 13_456 79.21(5) n
Si2 Er Si3 13_455 . 80.92(4) n
Si2 Er Si3 13_556 . 133.80(3) n
Si2 Er Si3 13_456 . 133.80(3) n
Si2 Er Si3 13 . 80.92(4) n
Ni Er Si3 13_556 . 96.08(2) n
Ni Er Si3 13_455 . 43.606(15) n
Ni Er Si3 13_456 . 96.08(2) n
Ni Er Si3 13 . 43.606(15) n
Si1 Er Si3 13_556 . 53.69(2) n
Si1 Er Si3 13_456 . 53.69(2) n
Si2 Er Si3 13_455 1_556 133.80(3) n
Si2 Er Si3 13_556 1_556 80.92(4) n
Si2 Er Si3 13_456 1_556 80.92(4) n
Si2 Er Si3 13 1_556 133.80(3) n
Ni Er Si3 13_556 1_556 43.606(15) n
Ni Er Si3 13_455 1_556 96.08(2) n
Ni Er Si3 13_456 1_556 43.606(15) n
Ni Er Si3 13 1_556 96.08(2) n
Si1 Er Si3 13_556 1_556 53.69(2) n
Si1 Er Si3 13_456 1_556 53.69(2) n
Si3 Er Si3 . 1_556 79.53(5) n
Si2 Er Si2 13_455 . 46.26(4) n
Si2 Er Si2 13_556 . 98.973(18) n
Si2 Er Si2 13_456 . 98.973(18) n
Si2 Er Si2 13 . 46.26(4) n
Ni Er Si2 13_556 . 136.343(15) n
Ni Er Si2 13_455 . 84.03(2) n
Ni Er Si2 13_456 . 136.343(15) n
Ni Er Si2 13 . 84.03(2) n
Si1 Er Si2 13_556 . 126.40(2) n
Si1 Er Si2 13_456 . 126.40(2) n
Si3 Er Si2 . . 100.61(3) n
Si3 Er Si2 1_556 . 179.85(3) n
Si2 Er Si2 13_455 1_556 98.973(18) n
Si2 Er Si2 13_556 1_556 46.26(4) n
Si2 Er Si2 13_456 1_556 46.26(4) n
Si2 Er Si2 13 1_556 98.973(18) n
Ni Er Si2 13_556 1_556 84.03(2) n
Ni Er Si2 13_455 1_556 136.343(15) n
Ni Er Si2 13_456 1_556 84.03(2) n
Ni Er Si2 13 1_556 136.343(15) n
Si1 Er Si2 13_556 1_556 126.40(2) n
Si1 Er Si2 13_456 1_556 126.40(2) n
Si3 Er Si2 . 1_556 179.85(3) n
Si3 Er Si2 1_556 1_556 100.61(3) n
Si2 Er Si2 . 1_556 79.24(5) n
Si2 Er Er 13_455 1_655 131.427(12) n
Si2 Er Er 13_556 1_655 48.573(12) n
Si2 Er Er 13_456 1_655 131.427(12) n
Si2 Er Er 13 1_655 48.573(12) n
Ni Er Er 13_556 1_655 49.754(7) n
Ni Er Er 13_455 1_655 130.246(7) n
Ni Er Er 13_456 1_655 130.246(8) n
Ni Er Er 13 1_655 49.754(7) n
Si1 Er Er 13_556 1_655 50.39(2) n
Si1 Er Er 13_456 1_655 129.61(2) n
Si3 Er Er . 1_655 90.0 n
Si3 Er Er 1_556 1_655 90.0 n
Si2 Er Er . 1_655 90.0 n
Si2 Er Er 1_556 1_655 90.0 n
Si2 Er Er 13_455 1_455 48.573(12) n
Si2 Er Er 13_556 1_455 131.427(12) n
Si2 Er Er 13_456 1_455 48.573(12) n
Si2 Er Er 13 1_455 131.427(12) n
Ni Er Er 13_556 1_455 130.246(8) n
Ni Er Er 13_455 1_455 49.754(7) n
Ni Er Er 13_456 1_455 49.754(7) n
Ni Er Er 13 1_455 130.246(8) n
Si1 Er Er 13_556 1_455 129.61(2) n
Si1 Er Er 13_456 1_455 50.39(2) n
Si3 Er Er . 1_455 90.0 n
Si3 Er Er 1_556 1_455 90.0 n
Si2 Er Er . 1_455 90.0 n
Si2 Er Er 1_556 1_455 90.0 n
Er Er Er 1_655 1_455 180.0 n
Si2 Er Er 13_455 13_456 50.86(3) n
Si2 Er Er 13_556 13_456 91.65(3) n
Si2 Er Er 13_456 13_456 50.86(3) n
Si2 Er Er 13 13_456 91.65(3) n
Ni Er Er 13_556 13_456 132.127(15) n
Ni Er Er 13_455 13_456 91.512(15) n
Ni Er Er 13_456 13_456 91.512(15) n
Ni Er Er 13 13_456 132.127(15) n
Si1 Er Er 13_556 13_456 170.31(2) n
Si1 Er Er 13_456 13_456 110.48(2) n
Si3 Er Er . 13_456 131.778(18) n
Si3 Er Er 1_556 13_456 131.778(18) n
Si2 Er Er . 13_456 48.114(18) n
Si2 Er Er 1_556 13_456 48.114(18) n
Er Er Er 1_655 13_456 119.914(6) n
Er Er Er 1_455 13_456 60.086(6) n
Si2 Er Er 13_455 13_556 91.65(3) n
Si2 Er Er 13_556 13_556 50.86(3) n
Si2 Er Er 13_456 13_556 91.65(3) n
Si2 Er Er 13 13_556 50.86(3) n
Ni Er Er 13_556 13_556 91.512(15) n
Ni Er Er 13_455 13_556 132.127(15) n
Ni Er Er 13_456 13_556 132.127(15) n
Ni Er Er 13 13_556 91.512(15) n
Si1 Er Er 13_556 13_556 110.48(2) n
Si1 Er Er 13_456 13_556 170.31(2) n
Si3 Er Er . 13_556 131.778(18) n
Si3 Er Er 1_556 13_556 131.778(18) n
Si2 Er Er . 13_556 48.114(17) n
Si2 Er Er 1_556 13_556 48.114(17) n
Er Er Er 1_655 13_556 60.086(6) n
Er Er Er 1_455 13_556 119.914(6) n
Er Er Er 13_456 13_556 59.827(12) n
Si2 Er Er 13_455 1_556 131.635(13) n
Si2 Er Er 13_556 1_556 48.365(13) n
Si2 Er Er 13_456 1_556 48.365(13) n
Si2 Er Er 13 1_556 131.635(13) n
Ni Er Er 13_556 1_556 49.554(8) n
Ni Er Er 13_455 1_556 130.446(8) n
Ni Er Er 13_456 1_556 49.554(8) n
Ni Er Er 13 1_556 130.446(8) n
Si1 Er Er 13_556 1_556 90.0 n
Si1 Er Er 13_456 1_556 90.0 n
Si3 Er Er . 1_556 129.77(2) n
Si3 Er Er 1_556 1_556 50.23(2) n
Si2 Er Er . 1_556 129.62(2) n
Si2 Er Er 1_556 1_556 50.38(2) n
Er Er Er 1_655 1_556 90.0 n
Er Er Er 1_455 1_556 90.0 n
Er Er Er 13_456 1_556 90.0 n
Er Er Er 13_556 1_556 90.0 n
Si2 Er Er 13_455 1_554 48.365(13) n
Si2 Er Er 13_556 1_554 131.635(13) n
Si2 Er Er 13_456 1_554 131.635(13) n
Si2 Er Er 13 1_554 48.365(13) n
Ni Er Er 13_556 1_554 130.446(8) n
Ni Er Er 13_455 1_554 49.554(8) n
Ni Er Er 13_456 1_554 130.446(8) n
Ni Er Er 13 1_554 49.554(8) n
Si1 Er Er 13_556 1_554 90.0 n
Si1 Er Er 13_456 1_554 90.0 n
Si3 Er Er . 1_554 50.23(2) n
Si3 Er Er 1_556 1_554 129.77(2) n
Si2 Er Er . 1_554 50.38(2) n
Si2 Er Er 1_556 1_554 129.62(2) n
Er Er Er 1_655 1_554 90.0 n
Er Er Er 1_455 1_554 90.0 n
Er Er Er 13_456 1_554 90.0 n
Er Er Er 13_556 1_554 90.0 n
Er Er Er 1_556 1_554 180.0 n
Si2 Ni Si3 . 13_455 120.29(5) n
Si2 Ni Si3 . 13 120.29(5) n
Si3 Ni Si3 13_455 13 119.42(9) n
Si2 Ni Si1 . 1_554 120.27(5) n
Si3 Ni Si1 13_455 1_554 75.27(3) n
Si3 Ni Si1 13 1_554 75.27(3) n
Si2 Ni Si1 . . 120.27(5) n
Si3 Ni Si1 13_455 . 75.27(3) n
Si3 Ni Si1 13 . 75.27(3) n
Si1 Ni Si1 1_554 . 119.46(9) n
Si2 Ni Er . 13_556 66.287(16) n
Si3 Ni Er 13_455 13_556 139.527(7) n
Si3 Ni Er 13 13_556 69.20(3) n
Si1 Ni Er 1_554 13_556 139.730(7) n
Si1 Ni Er . 13_556 69.05(3) n
Si2 Ni Er . 13_455 66.287(16) n
Si3 Ni Er 13_455 13_455 69.20(3) n
Si3 Ni Er 13 13_455 139.527(7) n
Si1 Ni Er 1_554 13_455 69.05(3) n
Si1 Ni Er . 13_455 139.730(7) n
Er Ni Er 13_556 13_455 132.57(3) n
Si2 Ni Er . 13 66.287(16) n
Si3 Ni Er 13_455 13 139.527(7) n
Si3 Ni Er 13 13 69.20(3) n
Si1 Ni Er 1_554 13 69.05(3) n
Si1 Ni Er . 13 139.730(7) n
Er Ni Er 13_556 13 80.892(15) n
Er Ni Er 13_455 13 80.493(15) n
Si2 Ni Er . 13_456 66.287(16) n
Si3 Ni Er 13_455 13_456 69.20(3) n
Si3 Ni Er 13 13_456 139.527(7) n
Si1 Ni Er 1_554 13_456 139.730(7) n
Si1 Ni Er . 13_456 69.05(3) n
Er Ni Er 13_556 13_456 80.493(15) n
Er Ni Er 13_455 13_456 80.892(15) n
Er Ni Er 13 13_456 132.57(3) n
Ni Si1 Ni 1_556 . 119.46(9) n
Ni Si1 Si1 1_556 9_556 120.27(5) n
Ni Si1 Si1 . 9_556 120.27(5) n
Ni Si1 Si3 1_556 13_556 52.22(3) n
Ni Si1 Si3 . 13_556 127.68(5) n
Si1 Si1 Si3 9_556 13_556 90.08(6) n
Ni Si1 Si3 1_556 13_455 127.68(5) n
Ni Si1 Si3 . 13_455 52.22(3) n
Si1 Si1 Si3 9_556 13_455 90.08(6) n
Si3 Si1 Si3 13_556 13_455 179.84(12) n
Ni Si1 Si3 1_556 13_456 52.22(3) n
Ni Si1 Si3 . 13_456 127.68(5) n
Si1 Si1 Si3 9_556 13_456 90.08(6) n
Si3 Si1 Si3 13_556 13_456 89.765(11) n
Si3 Si1 Si3 13_455 13_456 90.235(11) n
Ni Si1 Si3 1_556 13 127.68(5) n
Ni Si1 Si3 . 13 52.22(3) n
Si1 Si1 Si3 9_556 13 90.08(6) n
Si3 Si1 Si3 13_556 13 90.235(11) n
Si3 Si1 Si3 13_455 13 89.765(11) n
Si3 Si1 Si3 13_456 13 179.84(12) n
Ni Si1 Er 1_556 13_556 67.15(4) n
Ni Si1 Er . 13_556 67.15(4) n
Si1 Si1 Er 9_556 13_556 140.39(2) n
Si3 Si1 Er 13_556 13_556 63.20(4) n
Si3 Si1 Er 13_455 13_556 116.67(6) n
Si3 Si1 Er 13_456 13_556 116.67(6) n
Si3 Si1 Er 13 13_556 63.20(4) n
Ni Si1 Er 1_556 13_456 67.15(4) n
Ni Si1 Er . 13_456 67.15(4) n
Si1 Si1 Er 9_556 13_456 140.39(2) n
Si3 Si1 Er 13_556 13_456 116.67(6) n
Si3 Si1 Er 13_455 13_456 63.20(4) n
Si3 Si1 Er 13_456 13_456 63.20(4) n
Si3 Si1 Er 13 13_456 116.67(6) n
Er Si1 Er 13_556 13_456 79.21(5) n
Ni Si2 Si2 . 13 124.51(7) n
Ni Si2 Si2 . 13_455 124.51(7) n
Si2 Si2 Si2 13 13_455 110.98(15) n
Ni Si2 Er . 13_455 69.66(3) n
Si2 Si2 Er 13 13_455 137.91(3) n
Si2 Si2 Er 13_455 13_455 69.62(3) n
Ni Si2 Er . 13_556 69.66(3) n
Si2 Si2 Er 13 13_556 69.62(3) n
Si2 Si2 Er 13_455 13_556 137.91(3) n
Er Si2 Er 13_455 13_556 139.32(7) n
Ni Si2 Er . 13 69.66(3) n
Si2 Si2 Er 13 13 69.62(3) n
Si2 Si2 Er 13_455 13 137.91(3) n
Er Si2 Er 13_455 13 82.85(2) n
Er Si2 Er 13_556 13 83.27(3) n
Ni Si2 Er . 13_456 69.66(3) n
Si2 Si2 Er 13 13_456 137.91(3) n
Si2 Si2 Er 13_455 13_456 69.62(3) n
Er Si2 Er 13_455 13_456 83.27(3) n
Er Si2 Er 13_556 13_456 82.85(2) n
Er Si2 Er 13 13_456 139.32(7) n
Ni Si2 Er . . 140.38(2) n
Si2 Si2 Er 13 . 64.13(6) n
Si2 Si2 Er 13_455 . 64.13(6) n
Er Si2 Er 13_455 . 133.74(4) n
Er Si2 Er 13_556 . 81.027(18) n
Er Si2 Er 13 . 133.74(4) n
Er Si2 Er 13_456 . 81.027(18) n
Ni Si2 Er . 1_554 140.38(2) n
Si2 Si2 Er 13 1_554 64.13(6) n
Si2 Si2 Er 13_455 1_554 64.13(6) n
Er Si2 Er 13_455 1_554 81.027(18) n
Er Si2 Er 13_556 1_554 133.74(4) n
Er Si2 Er 13 1_554 81.027(18) n
Er Si2 Er 13_456 1_554 133.74(4) n
Er Si2 Er . 1_554 79.24(5) n
Ni Si3 Ni 13_455 13 119.42(9) n
Ni Si3 Si3 13_455 9_565 120.29(5) n
Ni Si3 Si3 13 9_565 120.29(5) n
Ni Si3 Si1 13_455 13_556 127.59(5) n
Ni Si3 Si1 13 13_556 52.51(3) n
Si3 Si3 Si1 9_565 13_556 89.92(6) n
Ni Si3 Si1 13_455 13_455 52.51(3) n
Ni Si3 Si1 13 13_455 127.59(5) n
Si3 Si3 Si1 9_565 13_455 89.92(6) n
Si1 Si3 Si1 13_556 13_455 179.84(12) n
Ni Si3 Si1 13_455 13_456 52.51(3) n
Ni Si3 Si1 13 13_456 127.59(5) n
Si3 Si3 Si1 9_565 13_456 89.92(6) n
Si1 Si3 Si1 13_556 13_456 89.765(11) n
Si1 Si3 Si1 13_455 13_456 90.235(11) n
Ni Si3 Si1 13_455 13 127.59(5) n
Ni Si3 Si1 13 13 52.51(3) n
Si3 Si3 Si1 9_565 13 89.92(6) n
Si1 Si3 Si1 13_556 13 90.235(11) n
Si1 Si3 Si1 13_455 13 89.765(11) n
Si1 Si3 Si1 13_456 13 179.84(12) n
Ni Si3 Er 13_455 1_554 67.19(4) n
Ni Si3 Er 13 1_554 67.19(4) n
Si3 Si3 Er 9_565 1_554 140.23(2) n
Si1 Si3 Er 13_556 1_554 117.02(6) n
Si1 Si3 Er 13_455 1_554 63.11(4) n
Si1 Si3 Er 13_456 1_554 117.02(6) n
Si1 Si3 Er 13 1_554 63.11(4) n
Ni Si3 Er 13_455 . 67.19(4) n
Ni Si3 Er 13 . 67.19(4) n
Si3 Si3 Er 9_565 . 140.23(2) n
Si1 Si3 Er 13_556 . 63.12(4) n
Si1 Si3 Er 13_455 . 117.02(6) n
Si1 Si3 Er 13_456 . 63.11(4) n
Si1 Si3 Er 13 . 117.02(6) n
Er Si3 Er 1_554 . 79.53(5) n
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Er Si2 13_455 2.9586(7) y
Er Si2 13_556 2.9586(7) n
Er Si2 13_456 2.9586(7) n
Er Si2 13 2.9586(7) n
Er Ni 13_556 3.0300(4) y
Er Ni 13_455 3.0300(4) n
Er Ni 13_456 3.0300(4) n
Er Ni 13 3.0300(4) n
Er Si1 13_556 3.0707(15) y
Er Si1 13_456 3.0707(15) n
Er Si3 . 3.0729(15) y
Er Si3 1_556 3.0729(15) n
Er Si2 . 3.0823(15) y
Er Si2 1_556 3.0823(15) n
Er Er 1_655 3.9152(5) y
Er Er 1_455 3.9152(5) n
Er Er 13_456 3.9254(6) y
Er Er 13_556 3.9254(6) n
Er Er 1_556 3.9313(6) y
Er Er 1_554 3.9313(6) n
Ni Si2 . 2.247(2) y
Ni Si3 13_455 2.2671(11) y
Ni Si3 13 2.2671(11) n
Ni Si1 1_554 2.2759(11) y
Ni Si1 . 2.2759(11) n
Ni Er 13_556 3.0300(4) n
Ni Er 13_455 3.0300(4) n
Ni Er 13 3.0300(4) n
Ni Er 13_456 3.0300(4) n
Si1 Ni 1_556 2.2759(11) n
Si1 Si1 9_556 2.340(4) y
Si1 Si3 13_556 2.7742(3) y
Si1 Si3 13_455 2.7742(3) n
Si1 Si3 13_456 2.7742(3) n
Si1 Si3 13 2.7742(3) n
Si1 Er 13_556 3.0707(15) n
Si1 Er 13_456 3.0707(15) n
Si2 Si2 13 2.376(2) y
Si2 Si2 13_455 2.376(2) n
Si2 Er 13_455 2.9586(7) n
Si2 Er 13_556 2.9586(7) n
Si2 Er 13 2.9586(7) n
Si2 Er 13_456 2.9586(7) n
Si2 Er 1_554 3.0823(15) n
Si3 Ni 13_455 2.2671(11) n
Si3 Ni 13 2.2671(11) n
Si3 Si3 9_565 2.347(4) y
Si3 Si1 13_556 2.7742(3) n
Si3 Si1 13_455 2.7742(3) n
Si3 Si1 13_456 2.7742(3) n
Si3 Si1 13 2.7742(3) n
Si3 Er 1_554 3.0729(15) n
